ORIGINAL ARTICLE

**Nobuo Sobue · Ian Woodhead**

## Improvement of simple impedance tomography method in RF range for

## estimating moisture distribution in squared timbers

**Abstract Improvement of the simple tomography method **

for estimating moisture distribution in squared timbers was conducted by using impedance measurement in the RF range at 250 kHz. The local impedance in the horizontal and vertical directions was measured during natural drying. An inverse procedure using a trial-and-error method was used to reconstitute the cross-sectional moisture distribution from the surface impedance measurement. Two essential corrections for the spatial heterogeneity of the electric fi eld between electrodes and for the calculation error due to the algorithm of the trial-and-error method were introduced to improve the accuracy of the reconstitution of the moisture distribution. The reconstituted moisture distribution matched well that determined by the oven-dry method.

**Key words Moisture distribution · Tomography method · **

Structural timber · Impedance measurement · RF range

### Introduction

Many types of electronic moisture meters are used in the wood industry. However, these meters are not suffi cient to detect the moisture gradient in structural timbers. A com-puter tomography method using X-rays has been studied for standing trees1 and for square timbers.2 Another method using neutron beam imaging has been studied for wood disks.3

These techniques can reproduce the cross-sectional moisture distribution, but they are too expensive to intro-duce into the wood industry. The other tomography method using impedance measurement has been studied in the high-frequency range4–8

and using direct current.9

From the point of view of improvement of the conventional electronic

N. Sobue (*)

Faculty of Agriculture, Shizuoka University, 836 Ohya, Suruga-ku, Shizuoka 422-8529, Japan

Tel. +81-54-238-4855; Fax +81-54-237-3028 e-mail: afnsobu@agr.shizuoka.ac.jp

I. Woodhead

Lincoln Venture Ltd., Lincoln, Christchurch 7640, New Zealand

meter, a pin-type sensing probe with multiple hollow elec-trodes indenting in a specimen has been designed for mea-suring the moisture gradient at different depths.10

Our fi nal target is application of the impedance tomography tech-nique in the radio frequency range to the inline grading of structural timbers with a low-cost moisture meter.

A recent study4

showed potential for estimating the cross-sectional moisture distribution in structural timber by using the impedance tomography method. However, the reconstitution of the moisture distribution was not ade-quate for practical commercial use. This work aims to improve the reconstitution of moisture distribution by con-sidering two kinds of signal correction. One corrects for the effect of the heterogeneity of the electric fi eld between the electrodes and the other corrects for the fl attening of the peak of the distribution pattern due to the inverse cal-culation algorithm used.

### Theory

Reconstitution of moisture content distribution

The algorithm used for the inverse calculation is commonly used for inverse problems in acoustic tomography and has the benefi t of simple calculation but with limited resolu-tion.11

In this article, the moisture distribution was
deter-mined so that the moisture content of individual cells in Fig.
1 satisfy Eq. 1 using the simple trial-and-error method.
Figure 1 shows the cross data table of 6 × 6 elements used
*to obtain the inverse solution. The value in each cell uij* is

*the local moisture content. UHj and UVi* are accumulated
moisture contents of the rows and the columns,
respectively:

*U* *i* *uij* *U* *u*

*j*

*j* *ij*

*i*

H = and V =

= =

### ∑

### ∑

1 6

1 6

(1)

The procedure for obtaining the solution is as follows:
In the fi rst step, an average value of each accumulated
*moisture content, UHi*, is distributed to each row cell:

′ =

*uij* *U*H*i* 6 (2)

In the second step, the average of the difference of the
accumulated moisture content in the column direction
*between UVj* and the fi rst estimated value is distributed to
each row cell:

′′ = ′ +⎛_{⎝⎜} − ′⎞_{⎠⎟}
=

### ∑

*uij* *uij* *U* *j* *uij*
*i*

V 1 6

6 (3)

This procedure is repeated in the row direction, and these two procedures are iterated until each value in the cross table converges to a stationary value. These series of inverse calculations were executed by an Excel (Microsoft) macro program.

### Materials and methods

*Boxed-heart squared green hemlock (Tsuga heterophylla) *
timber of 105 mm × 105 mm × 4 m was used. It was cut into
twelve short specimens of 320 mm and both ends were
sealed with silicone sealant. The specimens were dried
under room conditions in the temperature range 13°–20°C
and the average air dried density of the specimen was
490 kg/m3

. An impedance meter (Hioki-3531 Z HiTESTER)
*was used. The absolute value of the wood impedance Z was *
measured at 250 kHz with an excitation voltage of 1 V and
the electrode arrangement shown in Fig. 2. The local
imped-ance was measured by switching the detection electrode in
turn from positions 1 to 6. A pair of thin polyethylene sheets
was sandwiched between the electrodes and the timber.
After the electrical measurement, the specimen was cut into
36 (6 × 6) pieces to determine the moisture content
distribu-tion by an oven-dry method.

### Results and discussion

Fundamental equation converting impedance to moisture content

Past work4

showed that the impedance measurement at 250 kHz is appropriate for the moisture measurement because the impedance change due to the moisture content change is stable and large at this frequency.

Figure 3 shows the relationship between the impedance and the accumulated moisture content in the directions of the 6 rows and 6 columns for the pooled data through all drying stages, where the accumulated moisture content is defi ned as the sum of moisture contents in each row or column direction. There was no signifi cant difference between the regression equations for the row and column directions. Since these equations have acceptable correla-tion coeffi cients, the data in both row and column direccorrela-tions are pooled in the following analysis.

Corrections improving reconstitution of moisture distribution

It is well known and has been experimentally demonstrated that the temperature rise of timber piled between elec-trodes used for high-frequency drying of wood depends on the spatial position.12

Hence the strength of the electric fi eld between the electrodes shows a spatial heterogeneity.

Accordingly, prior to the reconstitution of the moisture distribution from the impedance data, the following two corrections were carried out: fi rst, the correction for heterogeneity of the electric fi eld in the cross section of the

*U*V6

*U*V5

*U*V4

*U*V3

*U*V2

*U*V1

*U*H6

*u*66

*u*65

*u*64

*u*63

*u*62

*u*61

*U*H5

*u*56

*u*55

*u*54

*u*53

*u*52

*u*51

*U*H4

*u*46

*u*45

*u*44

*u*43

*u*42

*u*41

*U*H3

*u*36

*u*35

*u*34

*u*33

*u*32

*u*31

*U*H2

*u*26

*u*25

*u*24

*u*23

*u*22

*u*21

*U*H1

*u*16

*u*15

*u*14

*u*13

*u*12

*u*11

*U*V6

*U*V5

*U*V4

*U*V3

*U*V2

*U*V1

*U*H6

*u*66

*u*65

*u*64

*u*63

*u*62

*u*61

*U*H5

*u*56

*u*55

*u*54

*u*53

*u*52

*u*51

*U*H4

*u*46

*u*45

*u*44

*u*43

*u*42

*u*41

*U*H3

*u*36

*u*35

*u*34

*u*33

*u*32

*u*31

*U*H2

*u*26

*u*25

*u*24

*u*23

*u*22

*u*21

*U*H1

*u*16

*u*15

*u*14

*u*13

*u*12

*u*11

**Fig. 1. Cross-sectional data table of 6 **× 6 elements of moisture content
*distribution. UHi and UVj* are the accumulated moisture contents in the

row and column directions, respectively

1 2 3 4 5 6 GE GE

Supply side electrode Detection side electrodes

**Fig. 2. Arrangement of the electrodes. GE, guard electrode**

ln(Z ) = -0.0087 U + 13.7277

R2 = 0.605

ln(Z )= -0.0083 U + 13.5619

R2_{ = 0.498}

10 11 12 13 14

0 100 200 300 400

Accumulated MC (%)

ln

(

*Z*

) (

Ω

)

**Fig. 3. Relationship between impedance ln(Z) and accumulated ***mois-ture content (MC) U of pooled data. Open circles, row direction; solid *
*circles, column direction; R*2_{, coeffi cient of determination; solid line, }

material, and second, the correction for the inverse calculation.

*Correction for heterogeneity of electric fi eld*

The fi rst correction is to compensate for the fi eld
heteroge-neity and it would depend on the spatial confi guration of
the electrodes, specimen size, and discontinuity of material
properties. For the particular geometrical conditions of this
experiment, the following two spatial groups were
consid-ered. One is made up of the outer rows and outer columns
*(U*V1*, U*V6*, U*H1*, and U*H6 in Fig. 1), and the other is made up
*of the core rows and columns (U*V2*–U*V5* and U*H2*–U*H5 in Fig.
1). The impedance versus moisture relationships were
obtained for these two distinct groups.

Figure 4 shows the relationship between the impedance

*Z and the accumulated moisture content U. The regression *

lines for the core group and outer group are as follows:

Core group: ln(*Z*core)= −0 0100*U*+14 112 *R* =0 635
2

. . . (4)

Outer group: ln(*Z*out)= −0 0151*U*+14 394 *R* =0 760
2

. . . (5)

*where R*2

is the coeffi cient of determination. The correlation coeffi cients were improved over those in Fig. 3 by separat-ing the data into the two groups.

The estimated values of the accumulated moisture
*content Z*EST in the core and outer parts are given by the
following equations inversely from Eqs. 4 and 5,
respectively:

*U*ESTcore=1411 2 100. − ln(*Z*core) (6)

*U*ESTout=953 2 66 23. − . ln(*Z*out) (7)

Figure 5 shows the relationship between the estimated
*accu-mulated moisture content U*EST for both row and column
directions and the oven-dry accumulated moisture content

*U*OVEN, and the regression equation is given by:

*U*OVEN=0 7522*U*EST+49 757 *R* =0 752

2

. . . (8)

*Although the equation fi ts the data reasonably well (R*2_{=}
0.752), the predicted moisture content is under-estimated
when below 200% and over-estimated when above 200%.

In order to correct this trend, the combination of the Eqs. 6–8 was altered as follows:

′ = − ( ) =

*U*ESTcore 1111 3 75 22ln *Z*core *R* 0 7523

2

. . . (9)

′ = − ( ) =

*U*ESTout 766 8 49 81ln *Z*out *R* 0 7523

2

. . . (10)

This treatment, while unorthodox for linear regression, addressed the nonlinearity inherent in the electric fi eld dis-tribution. The resulting relationship between the modifi ed moisture content and the oven-dry moisture content was given by:

*U*OVEN=*U*EST−0 0015 *R* =0 7523

2

. . (11)

The gradient of the regression line became 1, and there was no difference in the coeffi cient of determination from Eq. 8.

*Correction for algorithm in inverse calculation*

The second correction in the inverse calculation was also a development beyond the previous work,4

where the itera-tive method used was apt to fl atten the peak of the resolved distribution. The effect was quantitatively evaluated using the original data set obtained from the cross-sectional dis-tribution of the oven-dry moisture content. The original oven-dry moisture content data were compared with the reconstituted values to obtain the correction factors from eight data sets. The results were averaged and are shown in Fig. 6, which gives the magnitude of the correction factor applied to sharpen the moisture distribution. The correction factor in Fig. 6 shows that the uncorrected iteration method has a tendency to underestimate the core and four corner sections and to overestimate the remainder.

*Application of two corrections to impedance data*

The two corrections described above were adopted in the following order: fi rst, the corrections for spatial position given by Eqs. 9 and 10 were applied and then the correction

ln(Z

Z

)= -0.0100 U + 14.1116

R2 = 0.635

ln(Z ) = -0.0151U + 14.3941

R2

= 0.760 10

11 12 13 14

Accumulated MC (%)

0 100 200 300 400

ln

(

* *

) (

Ω

)

**Fig. 4. Effect of spatial location in the relationship between impedance **
*ln(Z) and U. Solid circles, core group; open circles, outer group*

U OVEN= 0.7522 UEST + 49.7569

R2

= 0.752

0 50 100 150 200 250 300 350

Estimated AMC (%)

Oven-dry AMC (%)

0 100 200 300 400

**Fig. 5. Relationship between oven-dry accumulated moisture content **
*U*OVEN* and estimated accumulated moisture content U*EST. AMC,

tionship of the local moisture contents between the oven-dry method and the reconstitution method was given by the following equation:

*u*OVEN =1 005*u*EST−0 582 *R* =0 713

2

. . . (12)

The deviation of Eq. 12 from the oven-dry results became large above the fi ber saturation point, but since the main object of the application is the moisture inspection of struc-tural timbers below the fi ber saturation point, the obtained results are suffi cient for practical evaluation of the moisture gradient of commercial timbers. The other important point is that the reconstituted cross-sectional moisture distribu-tion gives us useful informadistribu-tion to evaluate the drying process by determining whether the timber moisture content is within the target range to assure product quality. If a large moisture gradient remains in the timber, it may induce deg-radation such as checks and crooks during service. Figure 9 shows the relationship between the oven-dry average mois-ture content in the whole cross section and the predicted moisture content. The regression equation is as follows:

*U*whod=0 8678*U*whest+4 780 *R* =0 780

2

. . . (13)

An alternative regression line with zero intercept is as follows:

*U*whod=1 007*U*whest *R* =0 759

2

. . . (14)

The average moisture content is also well estimated by this tomography method.

1 _{2} _{3}

4 _{5}

6 S1

S2S3

S4S5

S6

-0.2 -0.15 -0.1 -0.05 0 0.05 0.1 0.15 0.2

Correction factor

Vertical position

Horizontal position

0.15-0.2 0.1-0.15 0.05-0.1 0-0.05 -0.05-0 -0.1--0.05 -0.15--0.1 -0.2--0.15

**Fig. 6. Correction factor per unit moisture content applied prior to **
inverse calculation

1 _{2}

3

4 _{5} _{S1}S2

S3

S4S5

S6

0 5 10 15 20 25 30 35 40

### Oven dry method

635-40 30-35 25-30 20-25 15-20 10-15 5-10 0-5

### No correction

1 _{2}

3 _{4}

5 _{6} S1S2

S3S4

S5S6

0 5 10 15 20 25 30 35 40

### After both corrections

1 _{2}

3 _{4}

5 _{6} S1

S2S3

S4S5

S6

0 5 10 15 20 25 30 35 40 1

2 _{3}

4

5 _{6} S1

S2S3

S4S5

S6

0 10 20 30 40 50 60

50-60 40-50 30-40 20-30 10-20 0-10

1 _{2}

3 _{4}

5 _{6} S1S2

S3S4

S5S6

0 10 20 30 40 50 60

1 _{2}

3 _{4}

5 _{6} S1

S2S3

S4S5

S6

0 10 20 30 40 50 60

Moisture content (%)

Vertical position

Horizontal position

**Fig. 7. Reconstituted moisture content (%) distributions. Left, oven-dry moisture content; middle, no correction; right, after both corrections**

for the inverse calculation procedure using the correction factor in Fig. 6 was adopted. Figure 7 shows the moisture content distributions for the oven-dry method and for the tomography method without corrections and after correc-tions. The prediction of moisture content distribution using the corrected inverse calculation showed a much closer alignment with the oven-dry results than those without the corrections.

rela-Further improvement to the described method would require another calculation algorithm that takes account of the curvilinear nature of the electric force lines. Introduc-tion of informaIntroduc-tion on diagonal elements such as by using X-ray computer tomography methods could be used, but these are complex and expensive. The advantages of the impedance measurement are not only low equipment and processing costs, but also safety and ease of handling in the fi eld and in the saw mill.

### Conclusions

The proposed method aimed at improvement of the recon-stitution of the moisture distribution in timber using

imped-ance measurements. Corrections for the effects of the heterogeneity of the electric fi eld and the inverse calcula-tion algorithm were introduced. The results showed better reconstitution of the local moisture contents of commercial timbers than the previous approach did. This method is a key technique leading to realization of a moisture meter estimating the cross-sectional moisture distribution in com-mercial timbers.

**Acknowledgment The authors wish to acknowledge Dr. Munehiro **
Date of the Kobayashi Institute of Physical Research for his advice on
the design of the electrodes and discussions.

### References

1. Kogure J, Kawamura H, Onoue M, Yamada H, Tsao JW (1984) Development of a portable X-ray computed tomographic scanner for measuring the annual rings of a live tree (in Japanese). Rigaku-Denki J 15:8–15

2. Kanagwa Y, Hattori Y (1985) Nondestructive measurement of moisture distribution in wood with a medical X-ray CT scanner II. Change in moisture distribution with drying (in Japanese). Mokuzai Gakkaishi 31:983–989

3. Nakanishi TM, Okano T, Karakama I, Ishihara T, Matsubayashi M (1998) Three-dimensional imaging of moisture in wood disk by neutron beam during drying process. Holzforschung 52:673–676 4. Sobue N, Inagaki M (2007) Estimation of cross-sectional moisture

content in commercial timbers by impedance measurement in RF range. In: Proceedings of 7th International Conference on Electro-magnetic Wave Interaction with Water and Moist Substances. Hamamatsu, Japan, April 15–18, pp 123–128

5. Suzuki Y (2007) Development of estimating method of moisture content of water distribution of Sugi (Japanese cedar) log using impedance measurements. In: Proceedings of 7th International Conference on Electromagnetic Wave Interaction with Water and Moist Substances. Hamamatsu, Japan, April 15–18, pp 107–113 6. Sobue N, Yokotsuka M (2003) Estimation of moisture gradient in

timbers by capacity measurement in RF range with scanning elec-trodes. In: Proceedings of 5th International Conference on Elec-tromagnetic Wave Interaction with Water and Moist Substances. Rotorua, New Zealand, March 23–26, pp 284–290

7. Titta M, Savolainen T, Lappalainen T (2003) Electrical impedance spectroscopy applications for wood moisture gradient measure-ment. In: Proceedings of 5th International Conference on Electro-magnetic Wave Interaction with Water and Moist Substances. Rotorua, New Zealand, March 23–26, pp 277–283

8. Sobue N (2000) Measurement of moisture gradient in wood by electrode scanning moisture analysis ESMA. In: Proceedings of 12th International Symposium on Nondestructive Testing of Wood. Sopron, Hungary, September 13–15, pp 301–306

9. Sakai M, Hashimoto A (1998) Continuous measurement of mois-ture distribution in lumber. In: Proceedings of Annual Meeting of Chubu Branch of Japan Wood Research Society in 1998 (in Japa-nese). Toyama, Japan, August 27, pp 40–41

10. Forrer JB (1984) An electronic system for monitoring gradients of drying wood. Forest Prod J 34(7/8):34–38

11. Menke W (1989) Discrete inverse theory. Academic Press Inc., San Diego (Japanese translation by Yanagitani T, Tsukada K, Kokin Shoin, Tokyo, pp 198–202)

12. Terazawa S (1994) All about kiln drying of wood (in Japanese). Kaiseisha, Otsu, p 54, 116

*u*OVEN = 1.005 *u*EST - 0.582

R2 = 0.713

0 10 20 30 40 50 60 70

0 20 40

Estimated MC (%)

60 80

Oven dry MC (%)

* Fig. 8. Relationship between u*OVEN

*and u*EST for individual positions

during all drying stages

Uwhod = 0.8678 Uwhest + 4.7985

R2 = 0.780

10 15 20 25 30 35 40 45 50

10 20 30 40 50

Estimated whole MC (%)

Oven dry whole MC (%)